1 INSTRUCTIONS Read all of the instructions and all of the questions before beginning the exam. There are 5 problems on this Final Exam, totaling 143 points. The tentative credit for each part is given to help you allocate your time accordingly. You have a total of 3 hours to finish this exam. Be careful not to spend all your time on any one part. This is a closed book exam, except you can have two two-sided sheet of notes and a calculator. Unless otherwise noted on a particular problem, you must show your work (in the space provided plus the backs of the pages, if needed) for all problems to receive full credit; simply providing answers will result in only partial or no credit, even if the answers are correct. If you require extra space beyond what is provided, be sure to turn in any material that is required to support your solutions. Note that there are extra pages at the end of this exam. Do not use any attached pages until you have exhausted the pages contained in this exam. Turn in the entire exam, including this cover sheet. Put your name on every page of this exam, as well as on any additional material that you submit. Be sure to provide units where necessary. Signature: Problem 1: Problem 2: Problem 3: Problem 4: Problem 5: Total: / 38 points / 25 points / 20 points / 25 points / 35 points / 143 points 1
2 Problem 1. Total 38 points Please provide short written answers to the questions that follow. (a) Which technology was the first in volume production, NMOS or PMOS, and why? (b) Are substrate doping levels higher or lower in modern (i.e., today s) CMOS versus 1990 s CMOS? Why? (c) A silicon wafer is uniformly doped with boron (to 2x10 15 cm -3 ) and phosphorus (to 1x10 15 cm -3 ) so that it is net p-type. This wafer is then thermally oxidized to grow about 1 µm of SiO 2. The oxide is then stripped and a measurement is made to determine the doping type of the wafer surface. Surprisingly it is found to be n-type. Explain why the surface was converted from p- to n-type. 2
3 Problem 1. (continued) (d) To etch aluminum, you use a solution composed of: 80% phosphoric acid (H 2 PO 4 ) + 5% nitric acid (HNO 3 ) + 5% acetic acid (CH 3 COOH) + 10% water (H 2 O) i) Explain the mechanism by which the above solution etches aluminum. ii) What is the biggest problem with use of this solution and how might you best solve it? (e) How does chemical mechanical polishing (CMP) differ from lapping? (f) Suppose you ran a CMOS process up to metal patterning and tested your devices before finishing the entire process just to see if the devices were functional. Suppose this test reveals that all of your threshold voltages are wrong. What should you do to fix this and how does your solution work? 3
4 Problem 1. (continued) (g) In LOCOS oxidation, patterned films of nitride on oxide are used to block oxidation over active area regions. Unfortunately, LOCOS also introduces bird s beaks that encroach into the active regions, and this limits how small an MOS device can be made. Can we suppress the bird s beak in LOCOS by dispensing with the oxide film and instead depositing nitride directly over silicon? What would be the problem with this approach? Explain. (h) Suppose you plan to use a stepper projection lithography tool to pattern polysilicon over oxide. The tool uses an exposure wavelength of 200 nm and has a numerical aperture of 0.5. What is the minimum theoretical feature size that this tool can resolve? What is the maximum height of topography over the wafer surface that this tool can handle while maintaining this resolution? 4
5 Problem 2. Total 25 points The cross-section for a standard, LOCOS-isolated, nwell CMOS technology (similar to the pwell process described in lecture) is shown below. (a) Label all layers in the process, including n+ and p+ diffusions. Also, delineate thermal oxides from LPCVD oxides. Then use wires (i.e., lines) and batteries to implement an inverter in this technology, hooking up relevant portions to V DD and ground, and clearly indicating inputs and outputs. (b) Draw on the figure the cross-section of a guard ring at a location that provides the most effective protection against latch-up. Indicate the dopant type used and the bias voltage to which this ring is attached. Explain why this location is better than any other. Draw parasitic transistors and current direction arrows to aid in your explanation 5
6 Problem 3. Total 20 points Boron ions are implanted into the SiO 2 -Silicon-SiO 2 sandwich structure shown below at a dose of cm -2. A subsequent high temperature step at 1000 o C for 4 hrs in a N 2 ambient is used to activate and drive-in the dopants. To simplify the problem, you can assume that the diffusion coefficient D boron (= m 2 /hr at 1000 o C) is the same in Si and SiO 2, that there is no boron segregation at the Si-SiO 2 interface, and that that implanted ranges of B + in silicon and SiO 2 are the same. SiO 2 Single Crystal Silicon 0.5 m 2 m SiO 2 Substrate (a) What is the implant energy that achieves the lowest possible sheet resistance in the silicon layer? (b) Estimate the sheet resistance. 6 More work space next page.
7 Problem 3. (continued) 7
8 Problem 4. Total 25 points The drain currents for four NMOSFETs on the same die with the same W drawn s (=50 m), but with different L drawn s, were measured for two different V GS s, with drain voltages set at 50mV, and sources and bulks tied to ground. The resulting data are summarized as follows: L drawn [ m] I d (V GS = 3V) [ A] I d (V GS = 6V) [ A] For this problem, assume that the effective channel width W eff = W drawn, the threshold voltage V t = 0.7V, and the gate oxide thickness X ox = 20nm, for all devices. Also assume that for a device with no external series resistance R ext, the drain current I d in the linear region (i.e., with small V DS ) is given approximately by ( ) ( ) Use the data and the graph paper below to determine the following parameters: (a) the external resistance in series with the channel, R ext (b) L = L drawn L eff, where L eff is the effective channel length considering all sources of deviation (c) the low field mobility, o ; and (d) of the devices. 8
9 Problem 4. (continued) 9 More work space next page.
10 Problem 4. (continued) 10
11 Problem 5. Total 35 points The simplified CMOS process flow used to fabricate an NMOS transistor is as follows: i) CMOS twin-well processing steps to form nwell s and pwell s, both with doping N sub =??? cm -3, and standard LOCOS to define active areas. ii) Sacrificial oxide growth: Target = 30 nm, 900 o C, 20 min. dry O 2. iii) Threshold implant: B11, E = 10 kev, D I =???cm -2. iv) Strip sacrificial oxide. v) Gate oxidation: 900 o C, 12 min. dry O min. N 2 anneal. Target = 10 nm. vi) Polysilicon gate deposition: 650 o C, 1 hr. 35 min. Target = 250 nm. vii) Gate definition. viii) Re-oxidation: 900 o C, 14 min. dry O min. N 2 anneal. Target = 20 nm SiO 2 on poly. ix) n+ S/D implant and anneal: 925 o C, 20 min. in N 2. x) p+ S/D implant. xi) PSG deposition: 450 o C. Target = 300 nm. xii) PSG densification: 925 o C, 20 min. wet O 2. xiii) Contact hole mask. xiv) Metal deposition, masking, and patterning. xv) Low temperature sintering. After fabricating an NMOS device using the above process flow, measurements are taken on the device to yield a plot of threshold voltage V t versus the square root of the inversion surface potential magnitude s plus V SB as shown below. V t [V] s + V SB [V 1/2 ] 11
12 Problem 5. (continued) In this problem, when calculating threshold voltages or determining effective dopant depths, use the approximation N s x s = Q, where Q is the effective implanted dose in the silicon, and x s is the effective depth of the implanted profile, assumed to have a constant dopant concentration of N tot = N s N sub. (Do not assume that N s =0.5N o ; rather, determine N s (or N tot ) from the experimental data.) Finally, assume that as an oxide grows over silicon, dopant atoms in the path of the oxide front end up in the oxide; those that are not reached by the oxide stay in the silicon. Answer the following questions. (a) Determine the effective depth of the threshold implant, x s. (b) Determine the threshold implant dose D I used in the above process. (c) Determine the background substrate concentration, N sub. 12 More work space next page.
13 Problem 5. (continued) 13 More work space next page.